LAYING FLOOR SCREEDS
LAYING FLOOR SCREEDS
page 02 1. INTRODUCTION
page 03 2. WHAT IS A SCREED?
page 04 3. TECHNICAL AND PERFORMANCE CHARACTERISTICS OF SCREEDS
page 07 4. TYPES OF SCREEDpage 07 4.1 UNBONDED SCREED
page 09 4.2 FLOATING SCREED
page 12 4.3 BONDED SCREED
page 13 4.4 HEATED SCREED
page 17 5. COMPOSITION OF SCREEDSpage 17 5.1 SPECIAL PRODUCTS FOR NORMAL-SETTING, RAPID-DRYING SCREEDS
page 19 5.2 SPECIAL PRODUCTS FOR RAPID-SETTING, RAPID-DRYING SCREEDS
page 20 5.3 ADVANTAGES OF SCREEDS MADE WITH MAPEI SPECIAL BINDERS AND PRE-BLENDED MORTARS COMPARED WITH TRADITIONAL SCREEDS
page 22 5.4 SUPER-PLASTICISING ADMIXTURES FROM THE MAPEFLUID RANGE FOR MIXING WITH WATER, CEMENT AND SUITABLE AGGREGATES
page 22 6. GENERAL GUIDELINES FOR LAYING SCREEDS
page 25 7. TYPICAL SCREED DEFECTS AND REPAIR PROCEDURES
1. INTRODUCTIONThe aim of this Technical Notebook is to define the fundamental criteria
to be considered when designing and laying screeds, and to highlight the
products available from MAPEI for laying durable screeds.
The service life and functionality of any type of flooring, whether the
material used is ceramic, stone, textile, resilient or wood, are highly
dependent on the physical and elastic-mechanical characteristics of
the substrate on which it is installed. These properties must be defined
according to a number of factors, such as the final use of the flooring,
which basically means the loads acting on its surface, environmental
conditions, the type of flooring to be installed, the compressibility of the
underlying layers and any deflections in the concrete floor slab.
LAYING FLOOR SCREEDS
2. WHAT IS A SCREED?A screed is a construction element laid in a range of thicknesses, and
its purpose is to bring the installation surface for the flooring to the
design height and to provide a surface suitable for installing the specified
flooring. Screeds are usually made from pre-blended mortar mixed with
cementitious binders or anhydrite-based binders. Depending on whether
it is laid directly on a supporting structure (for example a reinforced
concrete floor slab), on an isolating layer (for example a vapour barrier) or
on a layer of thermal insulation and/or soundproofing material, it is known
as a bonded, unbonded or floating screed. A screed may also have
an underfloor heating/cooling system incorporated within its structure
and, in such cases, is known as a heated screed.
When a screed is laid, it must mainly guarantee the following:
- that it forms a substrate suitable for installing the specified flooring;
- that it is laid on schedule;
- that its durability under various service conditions (laid internally
or externally, for civil, commercial or industrial flooring, etc.) is not
The durability of flooring, therefore, is influenced by the characteristics
of its substrate, which means the type of product selected to make
the substrate, the quality of preparation work, how it is laid and the
compactness and curing of the mix.
To sum up, when choosing which product to use to make the screed,
be it a special binder, a pre-blended mortar or traditional site-prepared
mortar, you must take into consideration the final use of the screed, site
conditions (internal or external, the thickness to be laid, etc.), the type of
flooring to be installed, the time to wait before installing the flooring and
the time required before putting the flooring into service.
3. TECHNICAL AND PERFORMANCE CHARACTERISTICS OF SCREEDSTo be suitable for installing flooring, the screed must have the following
- SUFFICIENT THICKNESS: its thickness depends on the type of
screed to be laid (see Section 4 Types of screed), and must be
sufficient for the type of flooring to be installed and the type/intensity
of traffic acting on it when in service.
- MECHANICALLY RESISTANT: its mechanical strength, as with
thickness, must be sufficient for the final use of the floor and for the type
of flooring to be installed. As a general rule, the mechanical strength of a
screed suitable for installing any type of flooring for domestic use must
be at least 20 MPa, while for industrial use it must be at least 30 MPa.
- COMPACT: the screed must be compact and homogeneous on
the surface and through the whole thickness. The presence of layers
or areas of crumbly, lower consistency is a sign of poor mechanical
characteristics which could cause breakage or detachment of the
flooring. These areas must be carefully assessed and, according to
the seriousness and extent of the defect, they must be removed and
repaired or consolidated with suitable products.
- CURED AND DIMENSIONALLY STABLE: before installing any type
of flooring, it is absolutely essential that the screed is cured and that
most of the shrinkage is completed. In fact, during the curing cycle,
screeds are prone to hygrometric shrinkage due to part of the mixing
water evaporating or drying off. This may cause curling or cracking
(Fig. 3.1 and Fig. 3.2). If cracks develop after installing the flooring (Fig.
3.3), the floor covering could be damaged and/or become detached.
LAYING FLOOR SCREEDS
Fig. 3.1 - Typical sail type deformation of an area of flooring subject to curling
Fig. 3.2 - Schematic diagram of cracks generated by curling in a square area
Configuration after deformation
The curing time for a traditional sand-cement screed is around 7-10
days per centimetre of thickness in good weather. Turnaround times
for a screed made from traditional cementitious mortar, therefore,
can be particularly long (more than 1 month). However, it is possible
to reduce curing times considerably by using special admixtures, or
by using special binders (such as MAPECEM or TOPCEM) or pre-
blended, controlled-shrinkage, rapid-drying and setting mortar (such
as MAPECEM PRONTO or TOPCEM PRONTO) in the mix.
- CRACK-FREE: there are a number of causes of cracks in screeds,
such as hygrometric shrinkage, too much water in the mix, the use of
aggregates which are too fine or too much cement. Before installing
flooring, all cracks must be monolithically sealed by filling them with
epoxy resin, such as EPORIP or EPOJET. If there are hairline cracks
on the surface of the screed, or if ceramic or stone flooring is to be
installed, it is possible to lay an anti-fracture membrane such as
MAPETEX on the screed.
- CLEAN: The surface of the screed must be perfectly clean. Dust, dirt,
detached areas, rubble and any other material or substance on the
surface of the screed must be removed before installing the flooring to
prevent compromising adhesion between the flooring and the screed
- DRY: The level of residual humidity in the screed must be checked. It
must conform to the maximum level for that type of floor covering and
must be uniform through the whole thickness of the screed, especially
when installing flooring sensitive to humidity. For cementitious-based
screeds, levels of less than 2% for wooden floors and less than
2.5-3% for PVC, rubber and linoleum are considered acceptable. For
anhydrite screeds, the level of residual humidity must be less than
0.5%, whatever type of floor covering is installed.
Fig. 3.3 - Serious damage caused by curling at an advanced state
Fig. 3.4 - Ceramic tile detached from a crumbly screed
The level of residual humidity in a screed is measured using an electric
or carbide hygrometer (Fig. 3.5).
- FLAT: flatness is checked by laying a straightedge at least 2 metres
long in all directions on the surface of the screed (Fig. 3.6). The
maximum acceptable tolerance with this particular straightedge is
2 mm, although the acceptable tolerance varies according to the
length of the straightedge used to check for flatness. If the flatness
is not in tolerance, the surface must be levelled off using a suitable
product before installing the flooring.
- SMOOTH: the suitability of the grade of finish of the surface and,
therefore, its level of roughness, depends on the type of flooring to
be installed. For example, a rough surface with open pores helps
the screed dry out and improves adhesion of skimming coats and
adhesives. If, on the other hand, a perfectly smooth, reflective finish is
required, for example when installing resilient flooring, it is advisable
to apply a skimming product designed specifically for this kind of use
on the surface of the screed.
LAYING FLOOR SCREEDS
Fig. 3.5 - The most reliable instrument to measure residual humidity in a screed is a carbide hygrometer
Fig. 3.6 - Method used to check the flatness of flooring
Negative deviation in flatness: within tolerance
Negative deviation in flatness: out of tolerance
4. TYPES OF SCREEDScreeds may be divided into the following types, depending on their